International Journal of Research in Advanced Engineering and Technology International Journal of Research in Advanced Engineering and Technology ISSN: 2455-0876 Impact Factor: RJIF 5.44 www.newengineeringjournal.in Volume 4; Issue 1; January 2018; Page No. 16-24 Comparative analysis of mix design method of concrete using fly ash Tanuj M.Tech, Construction and Real Estate Management, Deenbandhu Chhotu University of Science and Technology, Murthal Sonipat, Haryana, India Abstract Concrete is most widely used material which include cement as binding material. Fly Ash an industrial waste is rich in silica and being industrial waste it is difficult to dispose it Fly ash and presence of lime released by Hydration of cement act as binding, material Therefore Fly Ash can replace the cement. More will be Fly Ash used in concrete less will be the burden of pollution on the environment. This study was undertaken with to study available design methods incorporating Fly ash and suggest a most suitable one for future use. In order to achieve this objective the cubes were cast of M20, M25 and M30 of concrete by method of mix design i.e. IS10262: 1982, IS 10262:2009 and research paper by Shantanu Bhanja (January 2015). Keywords: cement, fly ash, strength, mix design Introduction Ordinary Portland Cement (PC) is widely used as a main building material; however, its manufacturing process results in a high emission of carbon dioxide (CO2) to the atmosphere (Metz et al., 2007; Sukmak et al., 2013). The production of cement is not environmental friendly as it damage nature in search of limestone and energy involved. Fly ash, also known as "pulverized fuel ash" in the United Kingdom, is a coal combustion product composed of fine particles that are driven out of the boiler with the flue gases. Fly Ash is an industrial waste. In India alone, we produce 75 million tons of fly ash every year, the disposal of which has become a serious environmental problem. The effective use of fly ash in concrete making is therefore attracting serious considerations of concrete technologists and government departments. fly ash includes substantial amounts of silicon dioxide (SiO2) (both amorphous and crystalline), aluminum oxide (Al2O3) and calcium oxide (Ca O). The more the percentage of amorphous silica high the quality and reactivity of Fly Ash which increase is strength. Therefore Fly Ash can replace the cement. More the Fly Ash used in concrete less will be the burden of pollution on environment. Material and Experimental Procedure Material Fly Ash: The source of fly ash is from the KHEDAR Power Plant in Haryana. The fly ash collected from the precipitators is used in concrete as it is the purest form of Fly Ash compared to other types. The chemical and physical tests were carried out on the Fly Ash sample. Table 1: Chemical composition of Fly Ash Parameter Test Method Results Units Chemical Analysis Silica content (SiO2) IS 1727:1967 61.86 % Silicon Dioxide + Aluminum Oxide + Iron Oxide IS 1727:1967 99.62 % Magnesium Oxide (MgO) IS 1727:1967 0.38 % Sulphuric Anhydroxide (SO3) IS 1727:1967 0.36 % Sodium Oxide (Na2O) IS 1727:1967 0.17 % Chloride Content (as Cl) IS 1727:1967 0.018 % Loss on Ignition IS 1727:1967 0.49 % Reactive Silica IS 1727:1967 35.32 % Physical Analysis Fineness ( Blaine’s Air Permeability ) IS 1727:1967 345 Kg/m2 Particle retained on 45 micron IS sieve (By Wet Sieving) IS 1727:1967 31 % Lime Reactivity IS 1727:1967 5.6 N/mm2 Compressive Strength at 28 days ( % of the strength of corresponding plain cement mortar cube ) IS 1727:1967 NA % Soundness ( Autoclave ) IS 1727:1967 0.07 % Total Parameters 13 16 International Journal of Research in Advanced Engineering and Technology Cement Ordinary Portland concrete (OPC) of 33 evaluation was utilized as a section of that the structure and properties is in consistence with the Indian standard association. Concrete will be defined as the holding material having strong and glue properties that create it capable to join the various development materials and structure the compacted get together. Standard/Normal Portland concrete is a standout amongst the most broadly utilised kind of Portland cement. Test performed for cement are as follows 1. Fineness Test Table 2: Fineness (As per IS: 4031- Prat-2) 1988 Sr. No. Item Sample 1 Sample 2 1. Sample taken in gm. 100 100 2. Passing through IS 90 micron sieve 98.72 99.10 3. Retained on IS 90 micron sieve 1.28 0.90 4. Fineness (%) 1.28 0.90 5. Average 1.09 2. Consistency of cement was found to be 28.5% 3. Setting time test Table 3: Setting Time as per (IS 4031 – Part 5) 1988 1. Initial setting time in minutes 2. Final setting time in minutes 128 mins 30 min. – 600 min. 245 mins Sand: The sand was purchased from local market of Sonipat which is generally Yamuna Sand 10 4.75 2.26 1.18 0.60 0.30 0.15 Wt. Retained 0 60 132 262 330 446 132 Comulative Weight % Wt.Retained Retained 0 0 60 4.29 192 13.71 454 32.43 774 55.23 1220 87.14 1352 96.57 % Wt. retained 0 8.13 90.32 97.88 Table 7 From the above results it can be observed that the maximum average compressive strength obtained was 16.66 MPa at 15% replacement of cement with fly ash. Therefore, the optimum quantity of fly ash that could be replaced with cement came to be 15% Further the experiments would be performed on 15% replacement of cement with fly ash. Ratio 100 58.88 58.65 8.65 Table 6: Grading of coarse aggregate (10 mm) Cummulative Weight Retained 0 1352 15012 16262 Determination of Optimum Quantity of Fly Ash In order to mix Fly Ash with concrete optimum quantity of Fly Ash was to be determined. The optimum quantity of fly ash was based on compressive testing of fly ash concret cubes at 5%, 15% and 25% were prepared and average compressive strength was noted as shown below. Nominal mix was prepared and was mixed in ratio 1:1:2 (M20). The compression testing was done on 7 days basis. 100 95.71 86.57 87.57 44.71 17.86 8.43 Table 5: Grading of coarse aggregate (20 mm) IS Wt. Sieve Retained 12.5 0 10 1352 4.75 13660 2.36 1250 Methodology The first step in methodology was to establish the properties of the material used. Further optimum Fly Ash content was determined so that Fly Ash can be added most efficiently and according to properties. After the determination of optimum Fly Ash content the mix was prepared according to three specified methods. 1. IS 10262:1982 2. IS 10262:2006 3. A research paper “Use of efficiency factor in mix proportioning of concrete” (Santanu Bhanja,2015) Ratio Coarse Aggregate: The coarse aggregate used in experiments were purchased from local market Kishanganj in Rajasthan IS Wt. Cumulative Weight % Wt. Sieve Retained Retained Retained 40 0 0 .0 20 1210 1246 6.42 10 15246 16456 27.35 4.75 2066 18522 92.35 Specific gravity of Coarse Aggregate (20 mm) = 2.82 The proportions of aggregate to be mixed was found to be 60% (20 mm) and 40% (10 mm) to obtain well graded aggregate as per IS 383:1970 requirements Fly Average Compressive Specimen1 Specimen 2 Specimen3 Ash Strength 5% 9.77 15.11 16.88 13.62 15% 16.88 17.77 15.35 16.66 25% 13.33 15.11 13.33 13.92 Table 4: Grading of sand (IS 383: 1970) IS Sieve Specific gravity of coarse aggregate (10 mm) = 2.67 Ratio 100 91.87 9.68 2.15 Result and Analysis The result and calculation include the calculation of various mix design using various methods, there strength and result is analyzed further Mix Proportions using IS 10262:2009 Mix Design (M20) [IS 10262:2009] 1. Stipulation of proportion Grade = M20 Type of cement = OPC33 Mineral Admixture = Fly Ash Max. size of Aggregate = 20 mm Workability = 100 mm (slump) Max w/c ratio = 0.45 Exposure = Mild 2. Test data of Material Cement – OPC33 (IS: 269) 17 International Journal of Research in Advanced Engineering and Technology Specific gravity 1. Cement = 3.15 2. Coarse aggregate = 2.61 3. Fine aggregate = 2.82 4. Fly Ash = 2.2 Water Absorption 1. Coarse Aggregate = 0.5% 2. Fine Aggregate = 1% Zone of fine aggregate = Zone 2 (IS383) 3. Target Strength of Mix Proportions Ft = fck +1.65D Ft = 20 + 1.65*4 (from table IS 10262:2009) Ft = 26.60 N/mm2 4. Selection of W/C Ratio: Assuming W/C ratio = 0.45 (Taking value from Fig. 1&2 from IS 10262:2009) 5. Selection of Water Content Max. water content for max. size of 20 mm aggregate = 186 liters For 100 mm slump = 186+6/100*186 = 197 liters 6. Calculation for Cement content W/C Ratio = 0.45 Cement + Fly Ash =197/0.45 = 438 kg/m3 >320 kg/m3 Hence ok Taking optimum quantity of Fly Ash and replacing same with cement Cementious material content = 15% of 438 =66 Hence, cement content = 372kg/m3 7. Proportion of CA and FA contents From table 3 (IS 10262:2009) For W/C = 0.45, Zone 2 of FA Volume of coarse aggregate = 0.62 Volume of fine aggregate = 1-0.62 = 0.38 8. Mix Calculations a) Volume of concrete = 1m3 b) Volume of cement = mass of cement/(specific gravity*1000) = 372/3.15*1/1000 = 0.118 cum c) Volume of fly ash = mass of fly ash/(specific gravity*1000) 66/2.2*1/1000 = 0.03 cum d) Volume of water = mass of water/(specific gravity*1000) 197/1000 = 0.197 cum e) Volume of all aggregate = [a-(b+c+d)] = [1-0.345] = 0.655 cum f) Mass of coarse aggregate = e* volume of ca* sp. gravity* 1000 = 0.655* 0.62*2.82*1000 = 1084 kg/m3 g) Mass of fine aggregate = 0.655*0.38*2.82*1000 = 702 k/m3 9. Mix Proportions Cement = 372 kg/m3 Fly ash = 66 kg/m3 Water = 197 kg/m3 Fine aggregate = 702 kg/m3 Coarse aggregate = 1084 kg/m3 W/C Ratio 0.45 Mix Design (M25) [IS 10262:2009] 1. Stipulations for proportions Grade = M25 type of cement = OPC 33 Minerals Admixture = fly ash Max size of aggregate = 20 mm Workability = 100 mm (slump) Max w/c ratio = 0.40 Min cement content 320 kg/m3 Exposure = Mild 2. Test data for Material Cement – OPC 33 (IS 269 Specific gravity 1. Cement = 3.15 2. Coarse aggregate = 2.67 3. Fine aggregate = 2.82 4. Fly ash = 2.2 Water absorption 1. Coarse aggregate = 0.5% 2. Fine aggregate = 1% Zone of fine aggregate = Zone 2 3. Target strength of mix proportions Ft = fck + 1.65D Ft = 25 + 1.65*4 [IS 10262:2009] Ft = 25 + 6.60 = 31.60 N/mm2 4. Selection of W/C Ratio Assuming W/C ratio = 0.40 (Taking value from Fig. 1&2 from IS 10262:2009) 5. Selection of Water Content Max. Water content for max. Size of 20 mm aggregate = 186 liters For 100 mm slump = 186+6/100*186 = 197 liters 6. Calculations of Cement and Fly Ash W/C ratio = 0.4 Cement + fly ash = 197/0.40 = 492 kg/m3 492 kg/m3 > 320 Hence OK Taking optimum quantity of fly ash and replacing the same with cement Cementious material content = 15% of 492 = 74 kg/m3 Hence cement content = 418 kg/m3 7. Proportion of CA and FA Content From table 3 (IS 10262:2009) For W/C = 0.45, Zone 2 of FA 18 International Journal of Research in Advanced Engineering and Technology Volume of coarse aggregate = 0.62 Volume of fine aggregate = 1-0.62 = 0.38 8. Mix Calculations a. Volume of concrete = 1m3 b. Volume of cement = mass of cement/(specific gravity*1000) 418/3.15*1/1000 = 0.133 cum c. Volume of fly ash = mass of fly ash/(specific gravity*1000) 74/2.2*1/1000 = 0.033 cum d. Volume of water = mass of water/(specific gravity*1000) 197/1*1/1000 = 0.197 cum e. Volume of all aggregate = [a-(b+c+d)] = 1 – 0.363 = 0.637 cum f. Mass of coarse aggregate = e* volume of ca* sp. gravity* 1000 0.637*0.62*2.67*1000 = 1054 kg/m3 9. Mix Proportions Cement = 418 kg/m3 Fly ash = 74 kg/m3 Water = 197 kg/m3 Fine aggregate = 682 kg/m3 Coarse aggregate = 1054 kg/m3 W/C Ratio 0.40 Mix Design (M30) [IS10262:2009] 1. Stipulations for proportions Grade = M25 Type of cement = OPC 33 Minerals Admixture = fly ash Max size of aggregate = 20 mm Workability = 100 mm (slump) Max w/c ratio = 0.40 Min cement content 320 kg/m3 Exposure = Mild 2. Test data for Material Cement – OPC 33 (IS 269) Specific gravity 1. Cement = 3.15 2. Coarse aggregate = 2.67 3. Fine aggregate = 2.82 4. Fly ash = 2.2 Water absorption 1. Coarse aggregate = 0.5% 2. Fine aggregate = 1% Zone of fine aggregate = Zone 2 3. Target strength of mix proportion Ft = fck + 1.65D [IS 10262:2009] Ft = 30 + 1.65*5 = 38.25 N/mm2 4. Selection of W/C Ratio Assuming W/C ratio = 0.35 (Taking value from Fig. 1&2 from IS 10262:2009) 5. Selection of water content Max. Water content for max. Size of 20 mm aggregate = 186 liters For 100 mm slump = 186+6/100*186 = 197 liters 6. Calculations of cement content W/C ratio = 0.4 Cement + fly ash = 197/0.40 = 492 kg/m3 492 kg/m3 > 320 Hence OK Taking optimum quantity of fly ash and replacing the same with cement Cementious material content = 15% of 492 = 74 kg/m3 Hence cement content = 418 kg/m3 7. Proportion of CA and FA Content From table 3 (IS 10262:2009) For W/C = 0.35, Zone 2 of FA Volume of coarse aggregate = 0.62 Volume of fine aggregate = 1-0.62 = 0.38 8. Mix Calculations a. Volume of concrete = 1m3 b. Volume of cement = mass of cement/(specific gravity*1000) 478/3.15*1/1000 = 0.15 cum c. Volume of fly ash = mass of fly ash/(specific gravity*1000) 85/2.2*1/1000 = 0.03 cum d. Volume of water = mass of water/(specific gravity*1000) 197/1*1/1000 = 0.197 cum e. Volume of all aggregate = [a-(b+c+d)] = 1 – 0.377 = 0.623 cum f. Mass of coarse aggregate = e* volume of ca* sp. gravity* 1000 0.623*0.62*2.67*1000 = 1031 kg/m3 g. Mass of fine aggregates 0.623*0.38*2.82*1000 = 668 kg/m3 9. Mix Proportions Cement = 478 kg/m3 Fly ash = 85 kg/m3 Water = 197 kg/m3 Fine aggregate = 668 kg/m3 Coarse aggregate = 1031 kg/m3 W/C Ratio 0.35 Table 8: Quantity of material Mix Cement Fly Ash Coarse aggregate Fine aggregate Water M20 372 66 1084 702 197 M25 418 74 1054 682 197 M30 478 85 1031 668 197 19 International Journal of Research in Advanced Engineering and Technology IS 10262 : 2009 Results Table 9: The following results were obtained from compressive strength test Designeattion M 20 M 25 M 30 Specimen 1 (MPa) 21.33 26.66 35.33 Specimen 2 (Mpa) 20.66 27.77 37.33 Specimen 3 (MPa) Average Compressive Strength (MPa) 21.33 21.10 26.22 26.88 37.55 36.69 Mix Proportion Using IS 10262:1986 Mix design for concrete of M20 Grade 1. Design stipulation a. Characterstics compressive strength required in field at 28 days = 20 N/mm2 b. Maximum size of aggregate = 20 mm c. Degree of workability = 0.9 compacting factor d. Degree of quality control = Good e. Type of exposure = Mild 2. Test data for material a. Cement used = OPC 33 grade b. Specific gravity: 1. Cement = 3.15 2. Coarse aggregate = 2.67 3. Fine aggregate = 2.82 c. Water absorption 1. Coarse aggregate = 0.5% 2. Fine aggregate = 1% Zone of fine aggregate = Zone 2 3. Target strength of mix proportion Ft = fck + 1.65 Ft = 20 + 1.65*4.6 = 27.6 N/mm2 4. Selection of W/C Ratio From fig. 1 the W/C ratio required for target mean strength of 27.6 MPa is 0.50 (This is lower than maximum value of 0.65 prescribed for 1978 t. Mild Exposure) 5. Selection of water & sand content From table 4 for 20 mm nominal maximum size aggregate and sand confirming to zone 2, water content per cubic meter of concrete = 197 kg Sand content by volume = 35% of total aggregate 6. Determination of cement and fly ash content W/C Ratio = 0.50 Cement = 186/0.5 = 372 kg/m3 (The cement content is adequate for mild exposure Acc. To Appendix A of IS 456) Replacements of cement by 15% fly ash Hence fly ash = 56 kg/m3 Final cement content = 316kg/m3 7. Determination of coarse and fine aggregate From table 3 for specified maximum size of aggregate of 20mm the amount of entrapped air in wet concrete is 2% 0.98 = [186+372/3.15+1/0.35*FA/2.82]*0.001 Fa = 667 kg/ m3 0.98 = [186+372/3.15+1/0.65*Ca/2.67] Ca = 1173 kg/m3 8. Mix Proportion 1. Cement = 316 kg/ m3 2. Fly Ash = 56 kg/ m3 3. Sand = 667 kg/ m3 4. Coarse aggregate = 1173 kg/ m3 5. Water = 197 kg/ m3 Mix design for concrete of M20 Grade 1. Design stipulation a. Characterstics compressive strength required in field at 28 days = 25 N/mm2 b. Maximum size of aggregate = 20 mm c. Degree of workability = 0.9 compacting factor d. Degree of quality control = Good e. Type of exposure = Mild 2. Test data for material d. Cement used = OPC 33 grade e. Specific gravity: 1. Cement = 3.15 2. Coarse aggregate = 2.67 3. Fine aggregate = 2.82 c. Water absorption 1. Coarse aggregate = 0.5% 2. Fine aggregate = 1% Zone of fine aggregate = Zone 2 3. Target strength of mix proportion: Ft = fck + 1.65D Ft = 25 + 1.65*5.3 = 33.74 N/mm2 4. Selection of W/C Ratio From fig. 1 the W/C ratio required for target mean strength of 33.74 MPa is 0.40 (This is lower than maximum value of 0.65 prescribed for 1978 t. Mild Exposure) 5. Selection of water & sand content From table 4 for 20 mm nominal maximum size aggregate and sand confirming to zone 2, water content per cubic meter of concrete = 197 kg Sand content by volume = 35% of total aggregate 20 International Journal of Research in Advanced Engineering and Technology 6. Determination of cement and fly ash content W/C Ratio = 0.40 Cement = 186/0.4 = 465 kg/m3 (The cement content is adequate for mild exposure Acc. To Appendix A of IS 456) Replacements of cement by 15% fly ash Hence fly ash = 70 kg/m3 Final cement content = 395 kg/m3 7. Determination of coarse and fine aggregate From table 3 for specified maximum size of aggregate of 20mm the amount of entrapped air in wet concrete is 2% 0.98 = [186+395/3.15+1/0.35*FA/2.82]*0.001 Fa = 660 kg/ m3 0.98 = [186+395/3.15+1/0.65*Ca/2.67] Ca = 1160 kg/m3 8. Mix Proportion a) Cement = 395 kg/ m3 b) Fly Ash = 70 kg/ m3 c) Sand = 660 kg/ m3 d) Coarse aggregate = 1160 kg/ m3 e) Water = 197 kg/ m3 Mix design for concrete of M30 Grade 1. Design stipulation a. Characteristics compressive strength required in field at 28 days = 30 N/mm2 b. Maximum size of aggregate = 20 mm c. Degree of workability = 0.9 compacting factor d. Degree of quality control = Good e. Type of exposure = Mild 2. Test data for material a. Cement used = OPC 33 grade b. Specific gravity: 1. Cement = 3.15 2. Coarse aggregate = 2.67 3. Fine aggregate = 2.82 c. Water absorption 1. Coarse aggregate = 0.5% 2. Fine aggregate = 1% Zone of fine aggregate = Zone 2 3. Target strength of mix proportion Ft = fck + 1.65D Ft = 30 + 1.65*6 = 39.9 N/mm2 4. Selection of W/C Ratio From fig. 1 the W/C ratio required for target mean strength of 39.9 MPa is 0.37 (This is lower than maximum value of 0.65 prescribed for 1978 t. Mild Exposure) 5. Selection of water & sand content From table 4 for 20 mm nominal maximum size aggregate and sand confirming to zone 2, water content per cubic meter of concrete = 197 kg Sand content by volume = 35% of total aggregate 6. Determination of cement and fly ash content W/C Ratio = 0.37 Cement = 186/0.37 = 503 kg/m3 (The cement content is adequate for mild exposure Acc. To Appendix A of IS 456) Replacements of cement by 15% fly ash Hence fly ash = 75 kg/m3 Final cement content = 428 kg/m3 7. Determination of coarse and fine aggregate From table 3 for specified maximum size of aggregate of 20mm the amount of entrapped air in wet concrete is 2% V=W+c/Sc+1/P*Fa/Sfa 0.98 = [186+428/3.15+1/0.35*FA/2.82]*0.001 Fa = 650 kg/ m3 V=W+c/Sc+1/(1-P)*Ca/Sca 0.98 = [186+428/3.15+1/0.65*Ca/2.67] Ca = 1142 kg/m3 8. Mix Proportion a. Cement = 428 kg/ m3 b. Fly Ash = 76 kg/ m3 c. Sand = 650 kg/ m3 d. Coarse aggregate = 1142 kg/ m3 e. Water = 197 kg/ m3 Table 10: Quantity of material Mix Cement Fly Ash Coarse aggregate Fine aggregate Water M20 316 56 1173 667 197 M25 395 70 1160 660 197 M30 438 75 1142 650 197 Results (IS 10262:1982) Table 11: The following results were obtained in compressive strength test Designation (MPa) Specimen 1 (MPa) Specimen 2 (MPa) M20 20.83 20.03 M25 24.84 25.50 M30 34.66 36.66 Use of Efficiency factor in Mix Proportioning of Fly Ash” Research Paper by Santanu Bhanja Specimen 3 (MPa) 19.77 25.70 35.77 Average compressive strength 20.20 25.33 35.14 21 International Journal of Research in Advanced Engineering and Technology The efficiency factor (k – value) is defined as part of pozzolonic material which can be considered as equivalent to Portland cement having the same properties as the concrete without pozzolonic material (k = 1 for Portland cement) Mix Design M20 [Research Paper by Dr. Santanu Bhanja] 1. Stipulation for Proportion Type of Cement = OPC 33 Minerals Admixtures = Fly Ash Max. size of aggregate = 20 mm Workability = 100 mm (slump) Exposure = Mild 2. Test Data for Material Cement – OPC33 (IS: 269) Specific gravity: 1. Cement = 3.15 2. Coarse aggregate = 2.61 3. Fine aggregate = 2.82 4. Fly Ash = 2.2 Water Absorption 1. Coarse Aggregate = 0.5% 2. Fine Aggregate = 1% Zone of fine aggregate = Zone 2 (IS383) 3. Target Strength of Mix Proportions Ft = fck +1.65D Ft = 20 + 1.65*4 (from table IS 10262:2009) Ft = 26.60 N/mm2 4. Selection of W/C Ratio Assuming W/C ratio = 0.45 (Taking value from Fig. 1&2 from IS 10262:2009) 5. Selection of Water Content Max. water content for max. size of 20 mm aggregate = 186 liters For 100 mm slump = 186+6/100*186 = 197 liters 6. Calculation for Cement content W/C Ratio = 0.45 Cement + Fly Ash =197/0.45 = 438 kg/m3 >320 kg/m3 Hence ok Taking optimum quantity of fly ash and replacing same with cement Cementious material content = 14.31% 14.31*438/100 = 63 kg/m3 Hence cement = 375 kg/m3 7. Proportion of CA and FA contents From table 3 (IS 10262:2009) For W/C = 0.45, Zone 2 of FA Volume of coarse aggregate = 0.62 Volume of fine aggregate = 1-0.62 = 0.38 8. Mix Calculations a. Volume of concrete = 1m3 b. Volume of cement = mass of cement/(specific gravity*1000) = 372/3.15*1/1000 = 0.119 cum c. Volume of fly ash = mass of fly ash/(specific gravity*1000) 66/2.2*1/1000 = 0.03 cum d. Volume of water = mass of water/(specific gravity*1000) 197/1000 = 0.197 cum e. Volume of all aggregate = [a-(b+c+d)] = [1-0.346] = 0.654 cum f. Mass of coarse aggregate = e. * volume of ca* sp. gravity* 1000 = 0.654* 0.62*2.82*1000 = 1083 kg/m3 9. Mix Proportions Cement = 375 kg/m3 Fly ash = 63 kg/m3 Water = 197 kg/m3 Fine aggregate = 701 kg/m3 Coarse aggregate = 1083 kg/m3 W/C Ratio 0.45 Mix Design M25 Research Paper by Dr. Santanu Bhanja 1. Stipulation for Proportion Type of Cement = OPC 33 Minerals Admixtures = Fly Ash Max. size of aggregate = 20 mm Workability = 100 mm (slump) Exposure = Mild 2. Test Data for Material Cement – OPC33 (IS: 269) Specific gravity: 1. Cement = 3.15 2. Coarse aggregate = 2.61 3. Fine aggregate = 2.82 4. Fly Ash = 2.2 Water Absorption 1. Coarse Aggregate = 0.5% 2. Fine Aggregate = 1% Zone of fine aggregate = Zone 2 (IS383) 3. Target Strength of Mix Proportions Ft = fck +1.65D Ft = 25 + 1.65*4 (from table IS 10262:2009) Ft = 31.60 N/mm2 4. Selection of W/C Ratio: Assuming W/C ratio = 0.40 (Taking value from Fig. 1&2 from IS 10262:2009) 5. Selection of Water Content Max. water content for max. size of 20 mm aggregate = 186 liters For 100 mm slump = 186+6/100*186 = 197 liters 6. Calculation for Cement content W/C Ratio = 0.40 Cement + Fly Ash =197/0.40 22 International Journal of Research in Advanced Engineering and Technology = 492 kg/m3 >320 kg/m3 Hence ok Taking optimum quantity of fly ash and replacing same with cement Cementious material content = 14.17% 14.17*492/100 = 74 kg/m3 Hence cement = 418 kg/m3 Zone of fine aggregate = Zone 2 (IS383) 7. Proportion of CA and FA contents From table 3 (IS 10262:2009) For W/C = 0.40, Zone 2 of FA Volume of coarse aggregate = 0.62 Volume of fine aggregate = 1-0.62 = 0.38 4. Selection of W/C Ratio Assuming W/C ratio = 0.35 (Taking value from Fig. 1&2 from IS 10262:2009) 8. Mix Calculations a. Volume of concrete = 1m3 b. Volume of cement = mass of cement/(specific gravity*1000) = 418/3.15*1/1000 = 0.133 cum c. Volume of fly ash = mass of fly ash/(specific gravity*1000) 74/2.2*1/1000 = 0.03 cum d. Volume of water = mass of water/(specific gravity*1000) 197/1000 = 0.197 cum e. Volume of all aggregate = [a-(b+c+d)] = [1-0.363] = 0.637 cum f. Mass of coarse aggregate = e* volume of ca* sp. gravity* 1000 = 0.637* 0.62*2.82*1000 = 1054 kg/m3 9. Mix Proportions Cement = 418 kg/m3 Fly ash = 74 kg/m3 Water = 197 kg/m3 Fine aggregate = 683 kg/m3 Coarse aggregate = 1054 kg/m3 W/C Ratio 0.40 Mix Design M30 [Research Paper by Dr. Santanu Bhanja] 1. Stipulation for Proportion Type of Cement = OPC 33 Minerals Admixtures = Fly Ash Max. size of aggregate = 20 mm Workability = 100 mm (slump) Exposure = Mild 2. Test Data for Material Cement – OPC33 (IS: 269) Specific gravity: 1. Cement = 3.15 2. Coarse aggregate = 2.61 3. Fine aggregate = 2.82 4. Fly Ash = 2.2 Water Absorption 1. Coarse Aggregate = 0.5% 2. Fine Aggregate = 1% 3. Target Strength of Mix Proportions Ft = fck +1.65D Ft = 30 + 1.65*5 (from table IS 10262:2009) Ft = 38.25 N/mm2 5. Selection of Water Content Max. water content for max. size of 20 mm aggregate = 186 liters For 100 mm slump = 186+6/100*186 = 197 liters 6. Calculation for Cement content W/C Ratio = 0.35 Cement + Fly Ash =197/0.35 = 563 kg/m3 >320 kg/m3 Hence ok Taking optimum quantity of fly ash and replacing same with cement Cementious material content = 13.8% 13.8*563/100 = 78 kg/m3 Hence cement = 485 kg/m3 7. Proportion of CA and FA contents From table 3 (IS 10262:2009) For W/C = 0.35, Zone 2 of FA Volume of coarse aggregate = 0.62 Volume of fine aggregate = 1-0.62 = 0.38 8. Mix Calculations a. Volume of concrete = 1m3 b. Volume of cement = mass of cement/(specific gravity*1000) = 478/3.15*1/1000 = 0.152 cum c. Volume of fly ash = mass of fly ash/(specific gravity*1000) 85/2.2*1/1000 = 0.038 cum d. Volume of water = mass of water/(specific gravity*1000) 197/1000 = 0.197 cum e. Volume of all aggregate = [a-(b+c+d)] = [1-0.387] = 0.613 cum f. Mass of coarse aggregate = e* volume of ca* sp. gravity* 1000 = 0.613* 0.62*2.82*1000 = 1014 kg/m3 9. Mix Proportions Cement = 485 kg/m3 Fly ash = 78 kg/m3 Water = 197 kg/m3 Fine aggregate = 656 kg/m3 Coarse aggregate = 1014 kg/m3 W/C Ratio 0.35 23 International Journal of Research in Advanced Engineering and Technology Table 12: Quantity of material Mix Cement Fly Ash Coarse aggregate M20 316 56 1083 M25 395 70 1054 M30 438 75 1014 Result by method suggested by S. Bhanja Table 13: Compressive strength of sample as follows Designatio Specimen Specimen Specimen Avg. Compressive n 1 2 3 Strength M20 22 21.33 20.88 23.70 M25 27.33 28.44 27.77 27.84 M30 37.33 35.77 37.55 36.88 Analysis of Result From the above three findings it can be seen that highest compressive strength is obtained through the mix design procedure suggested by Dr. Santanu Bhanja (2015). In this method properties of fly ash has been considered before designing the mix which is not in either of two design methods by Indian Standard i.e. IS 10262:2009 and IS 10262:1982. From the result presented above it is oblivious that compressive strength of concrete increase with increase of grade in all three methods. However, the compressive strength of cube is proportioned by IS 10262:2009 was higher by 4.50% for M20, 6.11% for M25 and 1.52% for M30 as compared to IS 10262:1982. The increase in strength of cubes proportioned by the method suggested by Bhanja had higher compressive strength by 12.32% for M20, 3.57% for M25 and 0.49% for M30 as compared to IS10262:2009. Moreover, the compressive strength was higher by 17.38% for M20, 9.90% M25 and 2.04% for M30 when compared to IS 10262:1982. It is therefore obvious that method suggested by Bhanja provided best result. As discussed by Singhal et.al 2013 IS 10262:1982 was best method when compared with COST (computer Optimization and software tool and ACI (American Concrete Institute Method) Therefore all these possible methods were tried with inclusion of fly ash. The cubes proportioned by the methods suggested by Bhanja had higher compressive strength since this method includes the property of fly ash as binding material which other method did not. It is therefore obvious that this method will be best to mix design concrete with fly ash. Fine aggregate 701 683 656 Water 197 197 197 Efficiency factor k 0.51 0.61 0.57 Reference 1. IS. 3812 (Part-I) – Specification for fly ash Bureau of Indian Standards, New Delhi. 2. Indian Standard, Ordinary Portland cement, 33 gradespecification, IS 269: Bureau of Indian Standards, 2000. 3. IS: 383 Specification for coarse and fine aggregates from natural sources for concrete, Bureau of Indian Standards, New Delhi, 1970. 4. IS: 10262 Recommended guidelines for concrete mix design, Bureau of Indian Standards, New Delhi, 1989. 5. IS. 10262 Concrete mix proportioning; Recommended Guidelines, Bureau of Indian Standards, New Delhi, 2009. 6. IS 4031: Physical tests of Ordinary Portland Cement Bureau of Indian Standards, New Delhi, 1988. 7. Bhanja S. Use of Efficiency factor in Mix Proportioning of Fly Ash Advances in Structural Engineering pp 17611771. Springer, 2015. 8. IS 1727: method for test of pozzolonic material Bureau of Indian Standard, 1967. 9. Kaushal K. Concrete Mix Design with Flyash & Superplasticizer ICI Bulletin June, 1997. 10. Zein Al-Abideen HM. Environmental impact on concrete practice. Concr. Int. 1998; 20(11):48-54. 11. Chindaprasirt P, Jaturapitakkul C, Chalee W, Rattanasak U. Comparative study on the characteristics of fly ash and bottom ash geopolymers, Waste Management. 2009; 29:539-543. 12. Saha S, Rajasekaran C. An experimental investigation to determine the properties of fly ash based geopolymers as per Indian Standards, in: Proceedings of Structural Engineering Convention, 21st–23rd December, Chennai, India, 2016, 646-651. Conclusion Based on the observations and discussion made in study following conclusion can be derived upon: 1. The mix proportion by IS 10262:2009 had better compressive strength than IS 10262:1982 2. The mix proportion IS 10262:2009 is therefore better than IS 10262:1982 method ACI method and COST method. 3. The method suggested by Bhanja is the best for mix proportioning of concrete which includes the properties fly ash in terms of efficiency factor. 24